Presentation on theme: "Estimating Crystallite Size Using XRD"— Presentation transcript:
1 Estimating Crystallite Size Using XRD MIT Center for Materials Science and EngineeringEstimating Crystallite Size Using XRDScott A Speakman, Ph.D.A
2 WarningThese slides have not been extensively proof-read, and therefore may contain errors.While I have tried to cite all references, I may have missed some– these slides were prepared for an informal lecture and not for publication.If you note a mistake or a missing citation, please let me know and I will correct it.I hope to add commentary in the notes section of these slides, offering additional details. However, these notes are incomplete so far.
3 Goals of Today’s Lecture Provide a quick overview of the theory behind peak profile analysisDiscuss practical considerations for analysisBriefly mention other peak profile analysis methodsWarren Averbach Variance methodMixed peak profilingwhole patternDiscuss other ways to evaluate crystallite sizeAssumptions: you understand the basics of crystallography, X-ray diffraction, and the operation of a Bragg-Brentano diffractometer
4 A Brief History of XRD 1895- Röntgen publishes the discovery of X-rays 1912- Laue observes diffraction of X-rays from a crystal1913- Bragg solves the first crystal structure from X-ray diffraction datawhen did Scherrer use X-rays to estimate the crystallite size of nanophase materials?Scherrer published on the use of XRD to estimate crystallite size in 1918, a mere 6 years after the first X-ray diffraction pattern was ever observed.Remember– nanophase science is not quite as new or novel as we like to think.
5 The Scherrer Equation was published in 1918 Peak width (B) is inversely proportional to crystallite size (L)P. Scherrer, “Bestimmung der Grösse und der inneren Struktur von Kolloidteilchen mittels Röntgenstrahlen,” Nachr. Ges. Wiss. Göttingen 26 (1918) ppJ.I. Langford and A.J.C. Wilson, “Scherrer after Sixty Years: A Survey and Some New Results in the Determination of Crystallite Size,” J. Appl. Cryst. 11 (1978) ppPaul Scherrer, “Determination of ?? and the inner structure of colloids using X-rays”,K is the Scherrer constant, lambda is the wavelength of X-radiation, theta is ½ the diffraction anglemore detail on the Scherrer equation later
6 X-Ray Peak Broadening is caused by deviation from the ideal crystalline lattice The Laue Equations describe the intensity of a diffracted peak from an ideal parallelopipeden crystalThe ideal crystal is an infinitely large and perfectly ordered crystalline arrayFrom the perspective of X-rays, “infinitely” large is a few micronsDeviations from the ideal create peak broadeningA nanocrystallite is not “infinitely” largeNon-perfect ordering of the crystalline array can includeDefectsNon-uniform interplanar spacingdisorder
7 As predicted by the Laue equations, the diffraction peaks becomes broader when N is not infinite N1, N2, and N3 are the number of unit cells along the a1, a2, and a3 directionsThe calculated peak is narrow when N is a large number (ie infinitely large)When N is small, the diffraction peaks become broaderA nanocrystalline phase has a small number of NThe peak area remains constant independent of NThe Scherrer equation is rooted in the peak profiles described by the Laue equationsWhen N1, N2, and N3 are large numbers, the three quotients are non-zero only when the Laue equations are closely satisfied; this produces a sharp peak (nearly a delta-function, see fig 3.2 on pg 30).When N1, N2, and N3 are not large numbers, the three quotients broaden. This is directly observed as broader peaks in the diffraction pattern.The area underneath the peak is constant, so that peak broadening is accompanied by a decrease in the maximum peak height
8 We cannot assume that all broad peaks are produced by nanocrystalline materials 6667686970717273742q(deg.)Intensity (a.u.)These two diffraction patterns come from the exact same sample (silicon).The apparent difference in peak broadening is due to the instrument optics, not due to specimen broadeningThese diffraction patterns were produced from the exact same sampleTwo different diffractometers, with different optical configurations, were usedThe apparent peak broadening is due solely to the instrumentation
9 Many factors may contribute to the observed peak profile Instrumental Peak ProfileCrystallite SizeMicrostrainNon-uniform Lattice DistortionsFaultingDislocationsAntiphase Domain BoundariesGrain Surface RelaxationSolid Solution InhomogeneityTemperature FactorsThe peak profile is a convolution of the profiles from all of these contributions
10 Before analysis, you must decide how you will define Peak Width 46.746.846.947.047.147.247.347.447.547.647.747.847.92q(deg.)Intensity (a.u.)Full Width at Half Maximum (FWHM)the width of the diffraction peak, in radians, at a height half-way between background and the peak maximumThis was most often used in older research because it is easier to calculateIntegral Breadththe total area under the peak divided by the peak heightthe width of a rectangle having the same area and the same height as the peakrequires very careful evaluation of the tails of the peak and the backgroundFWHM46.746.846.947.047.147.247.347.447.547.647.747.847.92q(deg.)Intensity (a.u.)
11 Integral Breadth may be the way to define peak width with modern analysis software Warren suggests that the Stokes and Wilson method of using integral breadths gives an evaluation that is independent of the distribution in size and shapeL is a volume average of the crystal thickness in the direction normal to the reflecting planesThe Scherrer constant K can be assumed to be 1Langford and Wilson suggest that even when using the integral breadth, there is a Scherrer constant K that varies with the shape of the crystallites
12 Other methods used to determine peak width These methods are used in more the variance methods, such as Warren-Averbach analysisMost often used for dislocation and defect density analysis of metalsCan also be used to determine the crystallite size distributionRequires no overlap between neighboring diffraction peaksVariance-slopethe slope of the variance of the line profile as a function of the range of integrationVariance-interceptnegative initial slope of the Fourier transform of the normalized line profile
13 Instrument and Sample Contributions to the Peak Profile must be Deconvoluted In order to analyze crystallite size, we must deconvolute:Instrumental Broadening FW(I)also referred to as the Instrumental Profile, Instrumental FWHM Curve, Instrumental Peak ProfileSpecimen Broadening FW(S)also referred to as the Sample Profile, Specimen ProfileWe must then separate the different contributions to specimen broadeningCrystallite size and microstrain broadening of diffraction peaksThis requires an Instrument Profile Calibration Curve
14 The Instrument Peak Profile Calibration Curve quantifies the contribution of the instrument to the observed peak widths47.047.247.447.647.82q(deg.)Intensity (a.u.)The peak widths from the instrument peak profile are a convolution of:X-ray Source ProfileWavelength widths of Ka1 and Ka2 linesSize of the X-ray sourceSuperposition of Ka1 and Ka2 peaksGoniometer OpticsDivergence and Receiving Slit widthsImperfect focusingBeam sizePenetration into the samplePatterns collected from the same sample with different instruments and configurations at MIT
15 Other Instrumental and Sample Considerations for Thin Films The irradiated area greatly affects the intensity of high angle diffraction peaksGIXD or variable divergence slits on the PANalytical X’Pert Pro will maintain a constant irradiated area, increasing the signal for high angle diffraction peaksboth methods increase the instrumental FWHMBragg-Brentano geometry only probes crystallite dimensions through the thickness of the filmin order to probe lateral (in-plane) crystallite sizes, need to collect diffraction patterns at different tiltsthis requires the use of parallel-beam optics on the PANalytical X’Pert Pro, which have very large FWHM and poor signal:noise ratios
16 In order to build a Instrument Peak Profile Calibration Curve Collect data from a standard using the exact instrument and configuration as will be used for analyzing the samplesame optical configuration of diffractometersame sample preparation geometryYou need a separate calibration curve for every different instrument and instrument configurationEven a small change, such as changing the divergence slit from ½ to ¼° aperture, will change the instrument profilecalibration curve should cover the 2theta range of interest for the specimen diffraction patterndo not extrapolate the calibration curveProfile fit the diffraction peaks from the standardFit the peak widths to a function such as the Cagliotti equation. Use this function as the calibration curve.
17 The Cagliotti equation describes how peak width varies with 2theta Hk is the Cagliotti function where U, V and W are refinable parameters
18 Selecting a standard for building the Instrument Peak Profile Calibration Curve Standard should share characteristics with the nanocrystalline specimenSimilar linear absorption coefficientsimilar mass absorption coefficientsimilar atomic weightsimilar packing densityThe standard should not contribute to the diffraction peak profilemacrocrystalline: crystallite size larger than 500 nmparticle size less than 10 micronsdefect and strain freeThere are several calibration techniquesInternal StandardExternal Standard of same compositionExternal Standard of different composition
19 Internal Standard Method for Calibration Mix a standard in with your nanocrystalline specimena NIST certified standard is preferreduse a standard with similar mass absorption coefficientNIST 640c SiNIST 660a LaB6NIST 674b CeO2NIST 675 Micastandard should have few, and preferably no, overlapping peaks with the specimenoverlapping peaks will greatly compromise accuracy of analysis
20 Internal Standard Method for Calibration Advantages:know that standard and specimen patterns were collected under identical circumstances for both instrumental conditions and sample preparation conditionsthe linear absorption coefficient of the mixture is the same for standard and specimenDisadvantages:difficult to avoid overlapping peaks between standard and broadened peaks from very nanocrystalline materialsthe specimen becomes contaminatedonly works with a powder specimen
21 External Standard Method for Calibration If internal calibration is not an option, then use external calibrationRun calibration standard separately from specimen, keeping as many parameters identical as is possibleThe best external standard is a macrocrystalline specimen of the same phase as your nanocrystalline specimenHow can you be sure that macrocrystalline specimen does not contribute to peak broadening?
22 Qualifying your Macrocrystalline Standard select powder for your potential macrocrystalline standardif not already done, possibly anneal it to allow crystallites to grow and to allow defects to healuse internal calibration to validate that macrocrystalline specimen is an appropriate standardmix macrocrystalline standard with appropriate NIST SRMcompare FWHM curves for macrocrystalline specimen and NIST standardif the macrocrystalline FWHM curve is similar to that from the NIST standard, than the macrocrystalline specimen is suitablecollect the XRD pattern from pure sample of you macrocrystalline specimendo not use the FHWM curve from the mixture with the NIST SRM
23 Disadvantages/Advantages of External Calibration with a Standard of the Same Composition will produce better calibration curve because mass absorption coefficient, density, molecular weight are the same as your specimen of interestcan duplicate a mixture in your nanocrystalline specimenmight be able to make a macrocrystalline standard for thin film samplesDisadvantages:time consumingdesire a different calibration standard for every different nanocrystalline phase and mixturemacrocrystalline standard may be hard/impossible to producecalibration curve will not compensate for discrepancies in instrumental conditions or sample preparation conditions between the standard and the specimen
24 External Standard Method of Calibration using a NIST standard As a last resort, use an external standard of a composition that is different than your nanocrystalline specimenThis is actually the most common method usedAlso the least accurate methodUse a certified NIST standard to produce instrumental FWHM calibration curveUse the standard that has the most similar linear absorption coefficient
25 Advantages and Disadvantages of using NIST standard for External Calibration only need to build one calibration curve for each instrumental configurationI have NIST standard diffraction patterns for each instrument and configuration available for download fromknow that the standard is high quality if from NISTneither standard nor specimen are contaminatedDisadvantagesThe standard may behave significantly different in diffractometer than your specimendifferent mass absorption coefficientdifferent depth of penetration of X-raysNIST standards are expensivecannot duplicate exact conditions for thin films
26 Consider- when is good calibration most essential? Broadening Due to Nanocrystalline SizeCrystallite SizeB(2q) (rad)FWHM (deg)100 nm0.00150.09950 nm0.00290.18210 nm0.01450.8715 nm0.02911.745FWHM of Instrumental Profileat 48° 2q0.061 degFor a very small crystallite size, the specimen broadening dominates over instrumental broadeningOnly need the most exacting calibration when the specimen broadening is small because the specimen is not highly nanocrystalline
27 What Instrument to Use?The instrumental profile determines the upper limit of crystallite size that can be evaluatedif the Instrumental peak width is much larger than the broadening due to crystallite size, then we cannot accurately determine crystallite sizeFor analyzing larger nanocrystallites, it is important to use the instrument with the smallest instrumental peak widthVery small nanocrystallites produce weak signalsthe specimen broadening will be significantly larger than the instrumental broadeningthe signal:noise ratio is more important than the instrumental profile
28 Comparison of Peak Widths at 47° 2q for Instruments and Crystallite Sizes ConfigurationFWHM (deg)Pk Ht to Bkg Ratio185mm radius, 0.5° DS, diffracted-beam monochromator, point detector0.124339240mm radius, 0.25° DS, beta-filter, linear PSD0.06081240mm radius, 0.5° DS, beta-filter, linear PSD0.07772240mm radius, 0.5° DS, diffracted-beam monochromator, linear PSD0.073111Gobel mirror, 0.09° Parallel Beam Collimator0.17550Gobel mirror, 0.27° Parallel Beam Collimator0.19455Crystallite SizeFWHM (deg)100 nm0.09950 nm0.18210 nm0.8715 nm1.745Instruments with better peak height to background ratios are better for small nanocrystallites, <20nmInstruments with smaller instrumental peak widths are better for larger nanocrystallites, >80 nm
29 For line profile analysis, must remove the instrument contribution to each peak list When analyzing the diffraction pattern from the sample, the instrument contribution to the peak width must be removedThe instrument contribution is convoluted with the specimen contribution to peak broadeningPeak deconvolution is a difficult process, so simpler calculations are often usedMost commonly, the observed peak width is treated as the sum of the instrument and specimen contributions𝐵 𝑜𝑏𝑠 = 𝐵 𝑠𝑝𝑒𝑐𝑖𝑚𝑒𝑛 + 𝐵 𝑖𝑛𝑠𝑡𝑟𝑢𝑚𝑒𝑛𝑡This works well when:crystallite size is the dominant contribution to peak broadeningThe peak broadening is largely Lorentzian in shapeOther analysis will treat the observed peak as the sum of the squares of the instrument and specimen contributions𝐵 𝑜𝑏𝑠 = 𝐵 𝑠𝑝𝑒𝑐𝑖𝑚𝑒𝑛 𝐵 𝑖𝑛𝑠𝑡𝑟𝑢𝑚𝑒𝑛𝑡 2microstrain is the dominant contribution to peak broadeningThe peak broadening is largely Gaussian in shape
30 Once the instrument broadening contribution has been remove, the specimen broadening can be analyzed Contributions to specimen broadeningCrystallite SizeMicrostrainNon-uniform Lattice DistortionsFaultingDislocationsAntiphase Domain BoundariesGrain Surface RelaxationSolid Solution InhomogeneityTemperature FactorsThe peak profile is a convolution of the profiles from all of these contributions
31 Crystallite Size Broadening Peak Width due to crystallite size varies inversely with crystallite sizeas the crystallite size gets smaller, the peak gets broaderThe peak width varies with 2q as cos qThe crystallite size broadening is most pronounced at large angles 2ThetaHowever, the instrumental profile width and microstrain broadening are also largest at large angles 2thetapeak intensity is usually weakest at larger angles 2thetaIf using a single peak, often get better results from using diffraction peaks between 30 and 50 deg 2thetabelow 30deg 2theta, peak asymmetry compromises profile analysis
32 The Scherrer Constant, K The constant of proportionality, K (the Scherrer constant) depends on the how the width is determined, the shape of the crystal, and the size distributionK actually varies from 0.62 to 2.08the most common values for K are:0.94 for FWHM of spherical crystals with cubic symmetry0.89 for integral breadth of spherical crystals w/ cubic symmetry1, because 0.94 and 0.89 both round up to 1For an excellent discussion of K, refer to JI Langford and AJC Wilson, “Scherrer after sixty years: A survey and some new results in the determination of crystallite size,” J. Appl. Cryst. 11 (1978) p
33 Factors that affect K and crystallite size analysis how the peak width is definedWhether using FWHM or Integral BreadthIntegral breadth is preferredhow crystallite size is definedthe shape of the crystalthe size distribution
34 How is Crystallite Size Defined Usually taken as the cube root of the volume of a crystalliteassumes that all crystallites have the same size and shapeNone of the X-ray diffraction techniques give a crystallite size that exactly matches this definitionFor a distribution of sizes, the mean size can be defined asthe mean value of the cube roots of the individual crystallite volumesthe cube root of the mean value of the volumes of the individual crystallitesScherrer method (using FWHM) gives the ratio of the root-mean-fourth-power to the root-mean-square value of the thicknessStokes and Wilson method (using integral breadth) determines the volume average of the thickness of the crystallites measured perpendicular to the reflecting planeThe variance methods give the ratio of the total volume of the crystallites to the total area of their projection on a plane parallel to the reflecting planes
35 The Stokes and Wilson method considers that each different diffraction peak is produced from planes along a different crystallographic directionStokes and Wilson method (using integral breadth) determines the volume average of the thickness of the crystallites measured perpendicular to the reflecting planeThis method is useful for identifying anisotropic crystallite shapes(002)a-axis// c-axis,// (200)
36 Remember, Crystallite Size is Different than Particle Size A particle may be made up of several different crystallitesCrystallite size often matches grain size, but there are exceptionsTEM images collected by Jane Howe at Oak Ridge National Laboratory.
37 The crystallite size observed by XRD is the smallest undistorted region in a crystal Dislocations may create small-angle domain boundariesDipolar dislocation walls will also create domain boundaries
38 Crystallite ShapeThough the shape of crystallites is usually irregular, we can often approximate them as:sphere, cube, tetrahedra, or octahedraparallelepipeds such as needles or platesprisms or cylindersMost applications of Scherrer analysis assume spherical crystallite shapesIf we know the average crystallite shape from another analysis, we can select the proper value for the Scherrer constant KAnistropic peak shapes can be identified by anistropic peak broadeningif the dimensions of a crystallite are 2x * 2y * 200z, then (h00) and (0k0) peaks will be more broadened then (00l) peaks.
39 Anistropic Size Broadening The broadening of a single diffraction peak is the product of the crystallite dimensions in the direction perpendicular to the planes that produced the diffraction peak.
40 Crystallite Size Distribution is the crystallite size narrowly or broadly distributed?is the crystallite size unimodal?XRD is poorly designed to facilitate the analysis of crystallites with a broad or multimodal size distributionVariance methods, such as Warren-Averbach, can be used to quantify a unimodal size distributionOtherwise, we try to accommodate the size distribution in the Scherrer constantUsing integral breadth instead of FWHM may reduce the effect of crystallite size distribution on the Scherrer constant K and therefore the crystallite size analysis
41 Values for K referenced in HighScore Plus Values of K from Langford and Wilson, J. Appl. Cryst (1978) are:0.94 for FWHM of spherical crystals with cubic symmetry0.89 for integral breadth of spherical crystals w/ cubic symmetry1, because 0.94 and 0.89 both round up to 1Assuming the Scherrer definition of crystallite size, values of K listed in the Help for HighScore Plus are:Crystallite ShapeFWHMIntegral BreadthSpheres0.891.07Cubes1.00 – 1.16Tetrahedra0.94 – 1.39Octahedra1.04 – 1.14
42 Limits for crystallite size analysis There is only broadening due to crystallite size when the crystallite is too small to be considered infinitely largeAbove a certain size, there is no peak broadeningThe instrument usually constrains the maximum size rather than this limit; this limit only matters for synchrotron and other high resolution instrumentsThe instrument contribution to the peak width may overwhelm the signal from the crystallite size broadeningIf the instrument profile is 0.120° with an esd of 0.001°, the maximum resolvable crystallite size will be limited byThe precision of the profile fitting, which depends on the peak intensity (weaker peaks give less precise widths) and noiseThe amount of specimen broadening should be at least 10% of the instrument profile widthIn practice, the maximum observed size for a standard laboratory diffractometer is 80 to 120 nmThe minimum size requires enough repeating atomic planes to produce the diffraction phenomenonThis depends on the size of the unit cellThe minimum size is typically between 3 to 10 nm, depending on the material
43 Microstrain Broadening lattice strains from displacements of the unit cells about their normal positionsoften produced by dislocations, domain boundaries, surfaces etc.microstrains are very common in nanoparticle materialsthe peak broadening due to microstrain will vary as:Ideal crystal𝜀= ∆𝑑 𝑑 (%)Distorted crystalcompare to peak broadening due to crystallite size:
44 Contributions to Microstrain Broadening Non-uniform Lattice DistortionsDislocationsAntiphase Domain BoundariesGrain Surface RelaxationOther contributions to broadeningfaultingsolid solution inhomogeneitytemperature factors
45 Non-Uniform Lattice Distortions Rather than a single d-spacing, the crystallographic plane has a distribution of d-spacesThis produces a broader observed diffraction peakSuch distortions can be introduced by:surface tension of nanoparticlesmorphology of crystal shape, such as nanotubesinterstitial impurities| | | | | | | | |26.527.027.528.028.529.029.530.02q(deg.)Intensity (a.u.)
46 Antiphase Domain Boundaries Formed during the ordering of a material that goes through an order-disorder transformationThe fundamental peaks are not affectedthe superstructure peaks are broadenedthe broadening of superstructure peaks varies with hkl
47 DislocationsLine broadening due to dislocations has a strong hkl dependenceThe profile is LorentzianCan try to analyze by separating the Lorentzian and Gaussian components of the peak profileCan also determine using the Warren-Averbach methodmeasure several orders of a peak001, 002, 003, 004, …110, 220, 330, 440, …The Fourier coefficient of the sample broadening will containan order independent term due to size broadeningan order dependent term due to strain
48 FaultingBroadening due to deformation faulting and twin faulting will convolute with the particle size Fourier coefficientThe particle size coefficient determined by Warren-Averbach analysis actually contains contributions from the crystallite size and faultingthe fault contribution is hkl dependent, while the size contribution should be hkl independent (assuming isotropic crystallite shape)the faulting contribution varies as a function of hkl dependent on the crystal structure of the material (fcc vs bcc vs hcp)See Warren, 1969, for methods to separate the contributions from deformation and twin faulting
49 Solid Solution Inhomogeneity Variation in the composition of a solid solution can create a distribution of d-spacing for a crystallographic planeSimilar to the d-spacing distribution created from microstrain due to non-uniform lattice distortionsCeO219 nm45464748495051522q(deg.)Intensity (a.u.)ZrO246nmCexZr1-xO20<x<1
50 Temperature FactorThe Debye-Waller temperature factor describes the oscillation of an atom around its average position in the crystal structureThe thermal agitation results in intensity from the peak maxima being redistributed into the peak tailsit does not broaden the FWHM of the diffraction peak, but it does broaden the integral breadth of the diffraction peakThe temperature factor increases with 2ThetaThe temperature factor must be convoluted with the structure factor for each peakdifferent atoms in the crystal may have different temperature factorseach peak contains a different contribution from the atoms in the crystal
51 Scherrer Analysis Calculates Crystallite Size based on each Individual Peak Profile Both crystallite size and microstrain can be calculated based on individual peak profiles IF you assume the other factor is insignificantTo test this assumption, look at how the calculated values vary over a long range of 2thetaIf the calculated crystallite size or microstrain is consistent over a large range of 2theta, this could indicate that the other factor can be ignoredYou cannot make this determination if you use a single diffraction peakIf crystallite size and/or microstrain varies as a function of 2theta, then additional analysis is required.If you have confirmed that crystallite size or microstrain is the only source of specimen broadening for a few samples from a family of specimens, then you MIGHT consider using only single diffraction peak for future analysis.
52 In this example, crystallite size is consistent over a long range of 2theta Crystallite size varies from 45 to 38 A from 28 to 95 degrees 2thetaThe average crystallite size is 4 nmXRD analysis is only precise to a nm level, not A as the software suggestsIn the future, we might use only 1 peak to analyze similar samplesPos. [°2Th.]FWHM Left [°2Th.]Integral Breadth [°2Th.]Crystallite Size only [Å]Micro Strain only [%]Shape Left28.376(2)1.328(5)1.00(2)32.929(9)1.52(3)1.00(5)47.261(5)1.48(1)0.98(2)56.119(5)1.62(2)0.95(5)58.85(2)1.6(1)0.9(2)69.14(1)1.75(5)0.6(3)76.42(1)1.88(4)1.0(1)78.80(2)1.96(8)1.0(2)88.12(1)2.05(7)1.0(3)95.10(1)2.3(1)1.0(4)
53 When both Crystallite Size and Microstrain vary as 2theta, then both are probably present When microstrain is present, the calculated “Crystallite Size only” will tend to decrease as a function of 2thetaWhen crystallite size broadening is present, the calculated “Microstrain only” will tend to decrease as a function of 2thetaPos. [°2Th.]FWHM Left [°2Th.]Integral Breadth [°2Th.]Crystallite Size only [Å]Micro Strain only [%]Shape Left(5)0.829(1)1.000(3)58.282(2)1.188(5)0.50(1)73.221(2)1.371(4)1.000(7)87.053(5)1.67(1)0.91(2)(5)2.18(2)0.99(2)
54 A lack of a systematic angular trend for crystallite size or microstrain indicates a more complex complicationPos. [°2Th.]FWHM Left [°2Th.]Integral Breadth [°2Th.]Crystallite Size only [Å]Micro Strain only [%]Shape Left(6)0.143(3)1.00(3)(4)0.118(1)0.74(2)(2)0.117(1)0.81(1)(3)0.119(1)0.79(2)(3)0.0990(9)0.82(1)43.523(1)0.200(5)0.86(4)(4)0.114(1)0.85(2)49.674(1)0.179(4)0.93(4)(8)0.112(3)1.00(4)52.368(1)0.119(3)(8)0.173(3)0.90(2)(3)0.108(1)0.92(1)
55 When both crystallite size and microstrain are present, a Williamson-Hall Plot is used Size broadeningMicrostrain broadeningy-interceptslope
56 When both crystallite size and microstrain are present, a Williamson-Hall Plot is used y-interceptslopeFW(S)*Cos(Theta)Sin(Theta)0.0000.7844.244*Fit Size/Strain: XS(Å) = 33 (1), Strain(%) = (0.0343), ESD of Fit = , LC = 0.751
57 Analysis Mode: Fit Size Only slope= 0= strainFW(S)*Cos(Theta)Sin(Theta)0.0000.7844.244*Fit Size Only: XS(Å) = 26 (1), Strain(%) = 0.0, ESD of Fit = , LC = 0.751
58 Analysis Mode: Fit Strain Only y-intercept= 0size= ∞FW(S)*Cos(Theta)Sin(Theta)0.0000.7844.244*Fit Strain Only: XS(Å) = 0, Strain(%) = (0.0112), ESD of Fit = , LC = 0.751
59 Analysis Mode: Fit Size/Strain Pos. [°2Th.]FWHM Left [°2Th.]Integral Breadth [°2Th.]Crystallite Size only [Å]Micro Strain only [%]Shape Left(5)0.829(1)1.000(3)58.282(2)1.188(5)0.50(1)73.221(2)1.371(4)1.000(7)87.053(5)1.67(1)0.91(2)(5)2.18(2)0.99(2)
60 Comparing Results Integral Breadth FWHM Size (A) Strain (%) ESD of Fit Size Only22(1)-0.011125(1)0.0082Strain Only4.03(1)0.03513.56(1)0.0301Size & Strain28(1)0.935(35)0.012532(1)0.799(35)0.0092Avg from Scherrer Analysis22.525.1
61 A large amount of crystallite size or microstrain will hinder analysis of the other term Both microstrain and crystallite size can be analyzed only when the broadening due to both is equivalentWhen the amount of microstrain is large, the maximum observable crystallite size will be limitedA 1% microstrain might limit the maximum crystallite size to as little as 40 nm. The small amount of broadening due to a larger crystallite size will not be accuratey quantifiedWhen the crystallite size is small, the maximum quantifiable microstrain will be limited
62 Other Ways of XRD Analysis Most alternative XRD crystallite size analyses use the Fourier transform of the diffraction patternVariance MethodWarren Averbach analysis- Fourier transform of raw dataConvolution Profile Fitting Method- Fourier transform of Voigt profile functionWhole Pattern Fitting in Fourier SpaceWhole Powder Pattern Modeling- Matteo Leoni and Paolo ScardiDirectly model all of the contributions to the diffraction patterneach peak is synthesized in reciprocal space from it Fourier transformfor any broadening source, the corresponding Fourier transform can be calculatedFundamental Parameters Profile Fittingcombine with profile fitting, variance, or whole pattern fitting techniquesinstead of deconvoluting empirically determined instrumental profile, use fundamental parameters to calculate instrumental and specimen profiles
63 Complementary Analyses TEMprecise information about a small volume of samplecan discern crystallite shape as well as sizePDF (Pair Distribution Function) Analysis of X-Ray ScatteringSmall Angle X-ray Scattering (SAXS)RamanAFMParticle Size Analysiswhile particles may easily be larger than your crystallites, we know that the crystallites will never be larger than your particles
64 Textbook ReferencesHP Klug and LE Alexander, X-Ray Diffraction Procedures for Polycrystalline and Amorphous Materials, 2nd edition, John Wiley & Sons, 1974.Chapter 9: Crystallite Size and Lattice Strains from Line BroadeningBE Warren, X-Ray Diffraction, Addison-Wesley, 1969reprinted in 1990 by Dover PublicationsChapter 13: Diffraction by Imperfect CrystalsDL Bish and JE Post (eds), Reviews in Mineralogy vol 20: Modern Powder Diffraction, Mineralogical Society of America, 1989.Chapter 6: Diffraction by Small and Disordered Crystals, by RC Reynolds, Jr.Chapter 8: Profile Fitting of Powder Diffraction Patterns, by SA Howard and KD PrestonA. Guinier, X-Ray Diffraction in Crystals, Imperfect Crystals, and Amorphous Bodies, Dunod, 1956.reprinted in 1994 by Dover Publications
65 ArticlesD. Balzar, N. Audebrand, M. Daymond, A. Fitch, A. Hewat, J.I. Langford, A. Le Bail, D. Louër, O. Masson, C.N. McCowan, N.C. Popa, P.W. Stephens, B. Toby, “Size-Strain Line-Broadening Analysis of the Ceria Round-Robin Sample”, Journal of Applied Crystallography 37 (2004)S Enzo, G Fagherazzi, A Benedetti, S Polizzi,“A Profile-Fitting Procedure for Analysis of Broadened X-ray Diffraction Peaks: I. Methodology,” J. Appl. Cryst. (1988) 21,“A Profile-Fitting Procedure for Analysis of Broadened X-ray Diffraction Peaks. II. Application and Discussion of the Methodology” J. Appl. Cryst. (1988) 21,B Marinkovic, R de Avillez, A Saavedra, FCR Assunção, “A Comparison between the Warren-Averbach Method and Alternate Methods for X-Ray Diffraction Microstructure Analysis of Polycrystalline Specimens”, Materials Research 4 (2) 71-76, 2001.D Lou, N Audebrand, “Profile Fitting and Diffraction Line-Broadening Analysis,” Advances in X-ray Diffraction 41, 1997.A Leineweber, EJ Mittemeijer, “Anisotropic microstrain broadening due to compositional inhomogeneities and its parametrisation”, Z. Kristallogr. Suppl. 23 (2006)BR York, “New X-ray Diffraction Line Profile Function Based on Crystallite Size and Strain Distributions Determined from Mean Field Theory and Statistical Mechanics”, Advances in X-ray Diffraction 41, 1997.
66 Instrumental Profile Derived from different mounting of LaB6 In analysis of Y2O3 on a ZBH, using the instrumental profile from thin SRM gives a size of 60 nm; using the thick SRM gives a size of 64 nm